Made of two or more different materials (such as sand, graphite, and metal) combining the advantages of each material. Used to improve mold strength, cooling rates and overall economics of the process.
Silica sand (Si O 2 ) is used more universally for making casting than any other molding materials.
* It is relatively cheap.
* It has good refractoriness.
A suitable bonding agent (usually clay) is mixed or occurs naturally with the sand; the mixture is moistened with water to develop strength and plasticity of the clay and to make the aggregate suitable for molding.
Sand refers to the molding material, the simplest type being a mixture of silica sand, clay and water, blended by hand or mechanical mixer .
The mold cavity is the empty shape left in sand when the pattern is removed and into which metal is poured, or cast, to form the casting.
The mold cavity may not be left completely empty; a core of firmly baked sand may be used to form the internal shape and dimensions of the casting.
Chaplets are metal objects for holding the core in position against the washing and lifting effect of molten metal.
Molten metal is introduced into the mold cavity through the gating system, which includes the downgate (sprue) and ingate . A pouring cup or pouring basin is either placed upon or formed into the upper cope surface, connecting to the downgate, to receive the metal from the ladle.
Green molding sand may be defined as a plastic mixture of sand grains, clay, water and other materials which can be used for molding and casting processes. The sand is called “green” because of the moisture present and is thus distinguished from dry sand.
The basic steps in green sand molding are the following:
Greater flexibility as a production process. Mechanical equipment can be utilized for performing molding and its allied operations. Furthermore, green sand can be reused many times by reconditioning it with water, clay and other materials.
Usually the most direct route from pattern to mold ready for pouring is green-sand molding.
Economy: Green sand molding is ordinarily the least costly method of molding unless special reasons exist which favor the other casting processes.
(i) Some casting designs can not be made and require the use of other casting processes. Thin, long projections of green sand in a mold cavity are washed away by the molten metal or may not even be moldable.
Cooling fins on air cooled engine cylinder blocks and heads are an example. Greater strength is then required of the mold.
(ii) Certain metals and some castings develop defects if poured into mold containing moisture.
(iv) The dimensional accuracy and surface finish of green-sand castings may not be adequate. A dimensional variation of ± 1/64 in. on small castings and ± 1/16 to ± 3/32 in. on larger ones may be encountered. However, this variation on many castings may be much less than that cited if adequate control is exercised.
(v) Large castings require greater mold strength and resistance to erosion than is available in green sands.
In making a simple mold, the bottom board is first laid securely on the bench or floor.
The pattern is positioned, the flask is located properly, and the sand is sieved over the pattern with a riddle. The sand employed for this purpose will touch the metal; in the best practice, it is an especially fine and clean variety of sand, called facing sand .
Used backing sand may then be shoveled into the flask over the facing, and the whole rammed securely, using the peen around the edges and the butt rammer over the pattern.
Once the flask is rammed properly a straightedge, or strike, is drawn across the upper surface to remove excess sand; a second flat board is placed upside down on the mold and flask and clamped or held in position while the whole is over-turned.
The original bottom board, which is now on the top, is removed, and the drag half of the mold is essentially finished.
It will later be necessary to cut an ingate to the mold cavity unless one is provided as part of the pattern, as is the recommended practice.
It may be necessary to tool the drag somewhat, i.e., smooth the sand around the pattern edges or otherwise shape it.
Parting powder, a white powdery substance, is dusted over the sand and pattern, and the cope flask is positioned.
If patterns are provided with downgates , these are set in place, as are the patterns for whatever risers are used. Downgates are sometimes cut through the cope with a cylindrical tube after the cope is finished.
A layer of facing sand is riddled over the drag and pattern as before, and backing sand is added and rammed solidly.
A steel bar is again used to strike off the upper surface of the cope; sprue and riser patterns are then drawn.
The cope is removed from the drag and usually placed aside for any finishing operations required.
If split patterns are used one-half will be picked up with the cope; so the cope is laid upside down on a spare bottom board.
The patterns are then rapped slightly to loosen them from the sand and are removed from cope and drag with a draw spike; ingates are cut, the mold is patched as required, chaplets and cores are positioned, and mold is closed by placing the cope again atop the drag.
Small vent holes are made through the sand to within a fraction of an inch of the pattern to insure the escape of gases.
Clamps or weights are placed on the flask to resist the tendency of the cope to float or shift as molten metal fills the mold cavity.
Figure: Basic steps involved in making a casting from a green sand mold.
The essential difference between dry sand and green sand molding is that the moisture in the mold sand is removed prior to pouring the metal.
Dry sand molding is more applicable to medium and large castings than to small castings.
The molds are stronger and more rigid than green sand molds. They can therefore withstand more handling and resist the static pressure of molten metal, which may cause green sand molds to deform or swell.
In addition, they may be exposed to the atmosphere for long periods of time without detrimental effect. Such exposure may be necessary for placing and fitting a large number of cores.
* Large intricate castings weighing from 1 to over 100 tons.
* The surface finish and dimensional accuracy of these large castings in ferrous alloys is not that of smaller ones, dimensional tolerances of ± 1/16 to ± ¼ in. being acceptable unless special experiences permits closer control.
* The problems of mold construction, handling, coring, gating, pouring and cleaning of large castings require much engineering efforts and control. The terrific amount of labor, time, and materials going into making a large casting makes the scrapping of one exceedingly costly.
* When the molds are medium to large in size, considerable heavy equipment, floor space and time must be allocated to the molding operation.
* Floor molding is done on the floor of bays of the foundry set aside for these heavy molding jobs.
When the pattern being molded is too large to be handled in flasks, the molding is done in pits.
Molding pits are concrete-lined box-shaped holes in the molding floor. The pattern is lowered into pit and molding sand is tucked and rammed under the pattern and up the side walls to the parting surface. The cope of the pit mold is finished off with cores or with sand rammed in a cope flask.
Figure: Dry sand pit mold for stationary diesel engine.
Floor molding : When castings increase in size, with resultant difficulty in handling, the work is done on the foundry floor. This type of molding is used for practically all medium and large size castings.
Pit molding : Extremely large castings are frequently molded in a pit instead of a flask. The pit acts as the drag part of the flask and a separate cope is used above it. They sides of the pit are brick kind, and on the bottom there.
* Loam is a molding sand containing about 50 per cent sand grains and 50 per cent clay.
* Loam molding was much used in the past for making large bronze castings and is still practiced in some shops, particularly in making huge manganese- bronze propellers.
* In this method a substrate is made of bricks, wood and other material to the approximate contour of the casting. A very viscous slurry of water, clay and sand is daubed over the framework and worked to proper shape with sweeps. The mold is dried by forced hot air or torches.
Cement-bonded molding sand is a mixture of sand, 8 to 12 per cent high-early-strength hydraulic cement, and 4 to 6 per cent water.
This sand develops great hardness and strength by the setting action of portland cement.
Molding may be performed by the methods discussed above and other specially suited to the cement.
The sand must be allowed to set or harden before the pattern can be with drawn. The mold is allowed to cure or continue setting for about 72 hours before the mold can be closed or assembled for pouring.
When the mold is poured, heat causes the water of crystallization of the cement to be driven off, and thus steam must be allowed to pass off through the sand by means of its porosity and suitably distributed vent holes.
Cement-bonded-sand molds can be constructed with considerable accuracy, often more than that obtainable in other processes for making large molds. Consequently more accurate castings may be obtained.
Some large castings are made entirely of cores; hundreds of large and small individual core sections are fitted together in a pit and finally rammed securely in position with molding sand or pressed together with suitable clamps.
Some large cores for this purpose weigh as much as 60 tons.
This method is chosen where design is such that standard patterns could not be drawn from regular molds.
In place of patterns, core boxes are used for making all parts of the mold.
The cores are being fitted together to make the mold, being located by alignment bosses and holes.
Skilled molders are not required, and process can be highly mechanized.
The sand used for shell molding consists of a mixture of the following ingredients:
Dry sand grains, AFS fineness 90 to 140, distributed over 4 to 5 screens. Sands for shell molding are always washed and graded for best results; fine sands can be used, as permeability of the thin shell is not a problem.
ii) The shell, still on the pattern, can then be cured by heating it to 550 to 650 F for 3 to 1 minute.
Stripping the shell from the mold presents a problem since the shell is very strong and grips the mold tightly. A mold release agent or parting agent is necessary so that the ejector pins can push the shell off the patterns.
Silicone parting solutions sprayed on the pattern have been found satisfactory.
The shell halves may then be assembled and poured.
Cleaning the mold by brushing or blasting with warm air, and maintaining them at proper casting temperature by a gas or oil flame; the correct operating temperature can be determined only by experience and varies with the casting;
Painting or spraying the mold surface with a thin refractory wash, or blacking it by depositing carbon from a reducing gas or oil flame;
Inserting cores, if used, and closing the mold by hand or by automatic action;
Pouring the metal from a hand ladle or a bull ladle suspended on a movable track;
Allowing sufficient time for the casting to solidify; and
Ejecting the casting from the mold automatically or by hand.
In submerged hot-chamber-type machine , molten metal flows into the hot chamber since it is submerged in the melt and is then forced into the die cavity at about 1000 to 2000 psi. This machine is used for casting Zn, Sn, Pb and other low melting alloys.
In gooseneck machine pressure may be applied directly by metal plunger or by air. The gooseneck may be filled by hand or it may be actuated by a cam to alternatively dip into the metal and rotate into the position against the die opening before pressure is applied for the shot.
* Lost-wax Process or Precision Casting or Lost Pattern
The term “investment” refers to a cloak or special covering apparel, in this case a refractory mold, surrounding a refractory-covered wax pattern.
In this process a wax pattern must be made for every casting and gating system to be cast; i.e., 100 casting require 100 patterns.
The patterns are cast by injection molding.
The basic steps involved in investment casting are as bellow:
A master pattern and die for casting the wax pattern is made. The die, usually a tin-bismuth alloy, must make allowance for shrinkage of both wax and later the metal casting, about 0.011 to 0.015 in. per in. total.
Wax patterns and gating systems are produced from the metal die. Wax employed are blends of beeswax, carnauba, ceresin, Acrawax, paraffin and other resins usually obtained as proprietary mixtures.
150 to 170 F and 500 to 1000 psi.
Polystyrene plastics ---- 300 to 600 F, 12,000 psi, iron or steel dies.
Mercury may also be used in place of wax patterns but must be frozen to retain the shape desired.
Patterns and gating system must be assembled if cast separately. They can be joined by heating the surfaces to be attached in the case of wax or moistening with a solvent, carbon tetrachloride, in case of polystyrene patterns.
(iii) Pre-coating: The wax assembly is dipped into a slurry of a refractory coating material. A typical slurry consists of 325-mesh silica flour suspended in water-ethyl silicate solution of suitable viscosity to produce a uniform coating after drying. After dipping the assembly is allowed to dry for up to 10 hours.
Sometimes pre-coating is not used and the wax pattern is directly invested in the molding material. In this case, the molding mixture must be vacuumed to remove air bubbles which may lodge next to the pattern.
( iv) The coated wax assembly is next invested in the mold. This is done by inverting the wax assembly on a table, surrounding it with a paper-lined steel flask, and pouring the investment-molding mixture around the pattern. The mold material settles by gravity and completely surrounds the pattern as the work table is vibrated.
The molding investment is composed of silica or quartz grains and binders. Two types of investments are used, one for low-temperature metals cast below 2000 F and others for metals with high pouring temperatures. The molds are allowed to air-set for 6 to 8 hours.
(v) Dewaxing and preheating: Wax is melted out of the hardened mold by heating it in an inverted position at 200 to 300 F. The wax may be reclaimed and reused. Molds with polystyrene patterns in them are preferably dried at 140 to 160 F. For burn out and preheating, the molds are heated at the rate of 100 to 160 F per hour from 1600 to 1900 F for ferrous alloys or 1200 F for aluminum alloys. The finishing temperature of preheating is controlled so that the mold is at a temperature desirable for pouring the particular alloy and casting design. Burnout and preheating cycle must completely eliminate wax and gas-forming material from the mold.
(vi) Pouring: In case of ferrous castings the mold is poured with metal from an individual small melting furnace, arc type, holding the exact weight required by the mold. When the metal is at pouring temperature the furnace and mold are inverted, transferring metal from the former to the latter. Air pressure may then be applied to the sprue to force-fill the mold cavity.
(vii) Cleaning operations follow cooling of the casting.
Casting high-pouring-temperature alloys to accurate dimensions.
Near net shape, excellent surface finish, minimum machining.
Castings of great exterior and interior intricacy may be cast.
Thin sections may be cast even, in the high-pouring-temperature alloys, because of the heated mold. Wires forms down to 0.002 in. in diameter and 2 in. long have been cast.
Casting in plaster molds, or plaster-bonded molds, has become a useful casting process.
Ag, Au, Mg, Cu,- and Al – base alloys may be cast in plaster molds, but ferrous alloys are not.
Plasters used for molding consist of mixtures of gypsum or plaster of Paris, CaSO 4 . ½ H 2 O, and ingredients such as talc, asbestos fiber, silica flour, and others to control the contraction characteristics of the mold and setting time.
The plaster is added to water and is mixed to a consistency of 140 to 180.
It is important that the plaster be added to water rather than water to plaster, and that an optimum rate of mixing be developed by experience for the particular mixer used; very rapid mixing develops too much air in the slurry, which adversely affects mold texture, and mixing too slowly may permit the slurry to harden (set) prematurely.
Consistency is defined as the pounds of water per 100 pounds of plaster in the mixture.
Dry strength of the plaster depends greatly on the consistency of the mix, as revealed in the table from R. F. Dalton.
After setting, the molds are dried at 400 F or higher. For aluminum castings, 10 to 20 hrs at 400 F is suitable.
The plaster can partially dehydrated at higher drying temperature, and consequently the mold evolves less steam when the casting are poured. However, mold strength is lost with dehydration.
It is obvious that the time required for curing plaster molds is an undesirable part of this process. However, because of dimensional accuracy and surface finish, many castings such as rubber-tier molds, foam-rubber molds, cast match plates, and the like are molded in this way.
A mixture of sand, gypsum, asbestos, talc, sodium silicate and water.
Sand is the bulk ingredient and gypsum the binder.
In proportions of 50 parts water to 100 parts dry ingredients, water is added to dry material consisting of 50 % silica sand, 40 % gypsum cement, 8 % talc, and small amount of sodium silicate, portland cement, and magnesium oxide .
Centrifugal force is used to distribute the molten metal in the mold.
Centrifugal casting falls into three categories:
1. True centrifugal casting
2. Semi-centrifugal casting
True centrifugal casting : the mold is spun about its own axis; no risers are required and no central core is needed since centrifugal force forms the inner diameter of castings such as pipe naturally.
Semi-centrifugal casting: the object, such as wheel with spokes, is spun about its own axis, but risers and cores are needed.
Centrifuged casting: the mold impressions are grouped around a central downgate, as in static casting, and centrifugal force is used mainly as a mold-filling device.
Centrifugal pressures ---- force molten metal quickly into mold to prevent premature freezing .
Centrifugal Casting Process Figure: Schematic illustration of the centrifugal casting process. Pipes, cylinder liners, and similarly shaped parts can be cast with this process.
Semicentrifugal Casting Figure: (a) Schematic illustration of the semicentrifugal casting process. Wheels with spokes can be cast by this process. (b) Schematic illustration of casting by centrifuging. The molds are placed at the periphery of the machine, and the molten metal is forced into the molds by centrifugal force.
Metal shots --- made by dropping molten metal from considerable heights into a pool of water.
The droplets become spherical in shape as they fall freely through air and freeze in this form upon striking the water.
Size of shot is regulated by type of metal, pouring temperature, rate of exit of metal stream, distance through which the droplets fall, and any air jet or mechanical device used to disperse the stream as it exits from the control nozzle.